The structure described by V8Ga3(MoS6)4 crystallizes in the triclinic P1 space group. There are eight inequivalent V sites. In the first V site, V(1) is bonded in a 6-coordinate geometry to one Mo(2), one S(1), one S(10), one S(14), one S(20), one S(23), and one S(7) atom. In the second V site, V(2) is bonded in a 6-coordinate geometry to one Mo(3), one S(11), one S(15), one S(2), one S(21), one S(24), and one S(8) atom. In the third V site, V(3) is bonded in a 6-coordinate geometry to one S(11), one S(13), one S(16), one S(2), one S(22), and one S(5) atom. In the fourth V site, V(4) is bonded in a 6-coordinate geometry to one Mo(2), one S(12), one S(14), one S(17), one S(23), one S(3), and one S(6) atom. In the fifth V site, V(5) is bonded in a 6-coordinate geometry to one Mo(3), one S(1), one S(10), one S(15), one S(18), one S(24), and one S(4) atom. In the sixth V site, V(6) is bonded in a 6-coordinate geometry to one S(1), one S(13), one S(16), one S(19), one S(4), and one S(7) atom. In the seventh V site, V(7) is bonded in a 6-coordinate geometry to one Mo(2), one S(14), one S(17), one S(2), one S(20), one S(5), and one S(8) atom. In the eighth V site, V(8) is bonded in a 6-coordinate geometry to one Mo(3), one S(15), one S(18), one S(21), one S(3), one S(6), and one S(9) atom. There are four inequivalent Mo sites. In the first Mo site, Mo(1) is bonded in a 6-coordinate geometry to one S(10), one S(16), one S(19), one S(22), one S(4), and one S(7) atom. In the second Mo site, Mo(2) is bonded in a 9-coordinate geometry to one V(1), one V(4), one V(7), one S(11), one S(17), one S(20), one S(23), one S(5), and one S(8) atom. In the third Mo site, Mo(3) is bonded in a 9-coordinate geometry to one V(2), one V(5), one V(8), one S(12), one S(18), one S(21), one S(24), one S(6), and one S(9) atom. In the fourth Mo site, Mo(4) is bonded in a 6-coordinate geometry to one S(12), one S(13), one S(19), one S(22), one S(3), and one S(9) atom. There are three inequivalent Ga sites. In the first Ga site, Ga(1) is bonded in a tetrahedral geometry to one S(1), one S(10), one S(5), and one S(9) atom. In the second Ga site, Ga(2) is bonded in a tetrahedral geometry to one S(11), one S(2), one S(6), and one S(7) atom. In the third Ga site, Ga(3) is bonded in a tetrahedral geometry to one S(12), one S(3), one S(4), and one S(8) atom. There are twenty-four inequivalent S sites. In the first S site, S(1) is bonded to one V(1), one V(5), one V(6), and one Ga(1) atom to form SV3Ga tetrahedra that share  a cornercorner with one S(10)V2GaMo tetrahedra,  a cornercorner with one S(5)V2GaMo tetrahedra,  a cornercorner with one S(9)VGaMo2 tetrahedra,  an edgeedge with one S(10)V2GaMo tetrahedra,  an edgeedge with one S(4)V2GaMo tetrahedra, and  an edgeedge with one S(7)V2GaMo tetrahedra. In the second S site, S(2) is bonded to one V(2), one V(3), one V(7), and one Ga(2) atom to form a mixture of corner and edge-sharing SV3Ga tetrahedra. In the third S site, S(3) is bonded to one V(4), one V(8), one Mo(4), and one Ga(3) atom to form SV2GaMo tetrahedra that share  a cornercorner with one S(4)V2GaMo tetrahedra,  a cornercorner with one S(8)V2GaMo tetrahedra,  a cornercorner with one S(12)VGaMo2 tetrahedra,  an edgeedge with one S(6)V2GaMo tetrahedra,  an edgeedge with one S(12)VGaMo2 tetrahedra, and  an edgeedge with one S(9)VGaMo2 tetrahedra. In the fourth S site, S(4) is bonded to one V(5), one V(6), one Mo(1), and one Ga(3) atom to form SV2GaMo tetrahedra that share  a cornercorner with one S(3)V2GaMo tetrahedra,  a cornercorner with one S(8)V2GaMo tetrahedra,  a cornercorner with one S(12)VGaMo2 tetrahedra,  an edgeedge with one S(10)V2GaMo tetrahedra,  an edgeedge with one S(7)V2GaMo tetrahedra, and  an edgeedge with one S(1)V3Ga tetrahedra. In the fifth S site, S(5) is bonded to one V(3), one V(7), one Mo(2), and one Ga(1) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(10)V2GaMo tetrahedra,  a cornercorner with one S(1)V3Ga tetrahedra,  a cornercorner with one S(9)VGaMo2 tetrahedra,  an edgeedge with one S(11)V2GaMo tetrahedra,  an edgeedge with one S(8)V2GaMo tetrahedra, and  an edgeedge with one S(2)V3Ga tetrahedra. In the sixth S site, S(6) is bonded to one V(4), one V(8), one Mo(3), and one Ga(2) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(11)V2GaMo tetrahedra,  a cornercorner with one S(7)V2GaMo tetrahedra,  a cornercorner with one S(2)V3Ga tetrahedra,  an edgeedge with one S(3)V2GaMo tetrahedra,  an edgeedge with one S(12)VGaMo2 tetrahedra, and  an edgeedge with one S(9)VGaMo2 tetrahedra. In the seventh S site, S(7) is bonded to one V(1), one V(6), one Mo(1), and one Ga(2) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(11)V2GaMo tetrahedra,  a cornercorner with one S(6)V2GaMo tetrahedra,  a cornercorner with one S(2)V3Ga tetrahedra,  an edgeedge with one S(10)V2GaMo tetrahedra,  an edgeedge with one S(4)V2GaMo tetrahedra, and  an edgeedge with one S(1)V3Ga tetrahedra. In the eighth S site, S(8) is bonded to one V(2), one V(7), one Mo(2), and one Ga(3) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(3)V2GaMo tetrahedra,  a cornercorner with one S(4)V2GaMo tetrahedra,  a cornercorner with one S(12)VGaMo2 tetrahedra,  an edgeedge with one S(11)V2GaMo tetrahedra,  an edgeedge with one S(5)V2GaMo tetrahedra, and  an edgeedge with one S(2)V3Ga tetrahedra. In the ninth S site, S(9) is bonded to one V(8), one Mo(3), one Mo(4), and one Ga(1) atom to form distorted SVGaMo2 tetrahedra that share  a cornercorner with one S(10)V2GaMo tetrahedra,  a cornercorner with one S(5)V2GaMo tetrahedra,  a cornercorner with one S(1)V3Ga tetrahedra,  an edgeedge with one S(3)V2GaMo tetrahedra,  an edgeedge with one S(6)V2GaMo tetrahedra, and  an edgeedge with one S(12)VGaMo2 tetrahedra. In the tenth S site, S(10) is bonded to one V(1), one V(5), one Mo(1), and one Ga(1) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(5)V2GaMo tetrahedra,  a cornercorner with one S(1)V3Ga tetrahedra,  a cornercorner with one S(9)VGaMo2 tetrahedra,  an edgeedge with one S(4)V2GaMo tetrahedra,  an edgeedge with one S(7)V2GaMo tetrahedra, and  an edgeedge with one S(1)V3Ga tetrahedra. In the eleventh S site, S(11) is bonded to one V(2), one V(3), one Mo(2), and one Ga(2) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(6)V2GaMo tetrahedra,  a cornercorner with one S(7)V2GaMo tetrahedra,  a cornercorner with one S(2)V3Ga tetrahedra,  an edgeedge with one S(5)V2GaMo tetrahedra,  an edgeedge with one S(8)V2GaMo tetrahedra, and  an edgeedge with one S(2)V3Ga tetrahedra. In the twelfth S site, S(12) is bonded to one V(4), one Mo(3), one Mo(4), and one Ga(3) atom to form distorted SVGaMo2 tetrahedra that share  a cornercorner with one S(3)V2GaMo tetrahedra,  a cornercorner with one S(4)V2GaMo tetrahedra,  a cornercorner with one S(8)V2GaMo tetrahedra,  an edgeedge with one S(3)V2GaMo tetrahedra,  an edgeedge with one S(6)V2GaMo tetrahedra, and  an edgeedge with one S(9)VGaMo2 tetrahedra. In the thirteenth S site, S(13) is bonded in a 3-coordinate geometry to one V(3), one V(6), and one Mo(4) atom. In the fourteenth S site, S(14) is bonded in a 3-coordinate geometry to one V(1), one V(4), and one V(7) atom. In the fifteenth S site, S(15) is bonded in a 3-coordinate geometry to one V(2), one V(5), and one V(8) atom. In the sixteenth S site, S(16) is bonded in a 3-coordinate geometry to one V(3), one V(6), and one Mo(1) atom. In the seventeenth S site, S(17) is bonded in a 3-coordinate geometry to one V(4), one V(7), and one Mo(2) atom. In the eighteenth S site, S(18) is bonded in a 3-coordinate geometry to one V(5), one V(8), and one Mo(3) atom. In the nineteenth S site, S(19) is bonded in a 3-coordinate geometry to one V(6), one Mo(1), and one Mo(4) atom. In the twentieth S site, S(20) is bonded in a 3-coordinate geometry to one V(1), one V(7), and one Mo(2) atom. In the twenty-first S site, S(21) is bonded in a 3-coordinate geometry to one V(2), one V(8), and one Mo(3) atom. In the twenty-second S site, S(22) is bonded in a 3-coordinate geometry to one V(3), one Mo(1), and one Mo(4) atom. In the twenty-third S site, S(23) is bonded in a 3-coordinate geometry to one V(1), one V(4), and one Mo(2) atom. In the twenty-fourth S site, S(24) is bonded in a 3-coordinate geometry to one V(2), one V(5), and one Mo(3) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_V8Ga3(MoS6)4
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   6.862
_cell_length_b   9.755
_cell_length_c   12.015
_cell_angle_alpha   65.655
_cell_angle_beta   72.932
_cell_angle_gamma   89.011
_symmetry_Int_Tables_number   1
_cell_volume   695.551
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  V  V0  1  0.412  0.006  0.192  1.0
  V  V1  1  0.746  0.339  0.525  1.0
  V  V2  1  0.931  0.536  0.140  1.0
  V  V3  1  0.271  0.865  0.474  1.0
  V  V4  1  0.604  0.198  0.808  1.0
  V  V5  1  0.791  0.395  0.999  1.0
  V  V6  1  0.128  0.723  0.334  1.0
  V  V7  1  0.463  0.058  0.666  1.0
  Ga  Ga8  1  0.004  0.999  0.000  1.0
  Ga  Ga9  1  0.338  0.332  0.333  1.0
  Ga  Ga10  1  0.672  0.665  0.665  1.0
  Mo  Mo11  1  0.207  0.400  0.998  1.0
  Mo  Mo12  1  0.530  0.735  0.333  1.0
  Mo  Mo13  1  0.863  0.069  0.666  1.0
  Mo  Mo14  1  0.071  0.669  0.864  1.0
  S  S15  1  0.728  0.136  0.000  1.0
  S  S16  1  0.061  0.469  0.333  1.0
  S  S17  1  0.396  0.803  0.666  1.0
  S  S18  1  0.578  0.438  0.848  1.0
  S  S19  1  0.909  0.773  0.183  1.0
  S  S20  1  0.242  0.106  0.515  1.0
  S  S21  1  0.426  0.287  0.151  1.0
  S  S22  1  0.757  0.621  0.484  1.0
  S  S23  1  0.092  0.956  0.817  1.0
  S  S24  1  0.275  0.136  0.000  1.0
  S  S25  1  0.607  0.470  0.334  1.0
  S  S26  1  0.940  0.804  0.665  1.0
  S  S27  1  0.735  0.626  0.004  1.0
  S  S28  1  0.084  0.958  0.333  1.0
  S  S29  1  0.419  0.292  0.666  1.0
  S  S30  1  0.909  0.286  0.173  1.0
  S  S31  1  0.234  0.617  0.511  1.0
  S  S32  1  0.567  0.950  0.844  1.0
  S  S33  1  0.083  0.452  0.825  1.0
  S  S34  1  0.411  0.795  0.156  1.0
  S  S35  1  0.745  0.128  0.489  1.0
  S  S36  1  0.261  0.632  0.005  1.0
  S  S37  1  0.590  0.972  0.333  1.0
  S  S38  1  0.922  0.305  0.666  1.0
[/CIF]
.
The structure described by V8Ga3(MoS6)4 crystallizes in the triclinic P1 space group. There are eight inequivalent V sites. In the first V site, V(1) is bonded in a 6-coordinate geometry to one Mo(2), one S(1), one S(10), one S(14), one S(20), one S(23), and one S(7) atom. In the second V site, V(2) is bonded in a 6-coordinate geometry to one Mo(3), one S(11), one S(15), one S(2), one S(21), one S(24), and one S(8) atom. In the third V site, V(3) is bonded in a 6-coordinate geometry to one S(11), one S(13), one S(16), one S(2), one S(22), and one S(5) atom. In the fourth V site, V(4) is bonded in a 6-coordinate geometry to one Mo(2), one S(12), one S(14), one S(17), one S(23), one S(3), and one S(6) atom. In the fifth V site, V(5) is bonded in a 6-coordinate geometry to one Mo(3), one S(1), one S(10), one S(15), one S(18), one S(24), and one S(4) atom. In the sixth V site, V(6) is bonded in a 6-coordinate geometry to one S(1), one S(13), one S(16), one S(19), one S(4), and one S(7) atom. In the seventh V site, V(7) is bonded in a 6-coordinate geometry to one Mo(2), one S(14), one S(17), one S(2), one S(20), one S(5), and one S(8) atom. In the eighth V site, V(8) is bonded in a 6-coordinate geometry to one Mo(3), one S(15), one S(18), one S(21), one S(3), one S(6), and one S(9) atom. There are four inequivalent Mo sites. In the first Mo site, Mo(1) is bonded in a 6-coordinate geometry to one S(10), one S(16), one S(19), one S(22), one S(4), and one S(7) atom. In the second Mo site, Mo(2) is bonded in a 9-coordinate geometry to one V(1), one V(4), one V(7), one S(11), one S(17), one S(20), one S(23), one S(5), and one S(8) atom. In the third Mo site, Mo(3) is bonded in a 9-coordinate geometry to one V(2), one V(5), one V(8), one S(12), one S(18), one S(21), one S(24), one S(6), and one S(9) atom. In the fourth Mo site, Mo(4) is bonded in a 6-coordinate geometry to one S(12), one S(13), one S(19), one S(22), one S(3), and one S(9) atom. There are three inequivalent Ga sites. In the first Ga site, Ga(1) is bonded in a tetrahedral geometry to one S(1), one S(10), one S(5), and one S(9) atom. In the second Ga site, Ga(2) is bonded in a tetrahedral geometry to one S(11), one S(2), one S(6), and one S(7) atom. In the third Ga site, Ga(3) is bonded in a tetrahedral geometry to one S(12), one S(3), one S(4), and one S(8) atom. There are twenty-four inequivalent S sites. In the first S site, S(1) is bonded to one V(1), one V(5), one V(6), and one Ga(1) atom to form SV3Ga tetrahedra that share  a cornercorner with one S(10)V2GaMo tetrahedra,  a cornercorner with one S(5)V2GaMo tetrahedra,  a cornercorner with one S(9)VGaMo2 tetrahedra,  an edgeedge with one S(10)V2GaMo tetrahedra,  an edgeedge with one S(4)V2GaMo tetrahedra, and  an edgeedge with one S(7)V2GaMo tetrahedra. In the second S site, S(2) is bonded to one V(2), one V(3), one V(7), and one Ga(2) atom to form a mixture of corner and edge-sharing SV3Ga tetrahedra. In the third S site, S(3) is bonded to one V(4), one V(8), one Mo(4), and one Ga(3) atom to form SV2GaMo tetrahedra that share  a cornercorner with one S(4)V2GaMo tetrahedra,  a cornercorner with one S(8)V2GaMo tetrahedra,  a cornercorner with one S(12)VGaMo2 tetrahedra,  an edgeedge with one S(6)V2GaMo tetrahedra,  an edgeedge with one S(12)VGaMo2 tetrahedra, and  an edgeedge with one S(9)VGaMo2 tetrahedra. In the fourth S site, S(4) is bonded to one V(5), one V(6), one Mo(1), and one Ga(3) atom to form SV2GaMo tetrahedra that share  a cornercorner with one S(3)V2GaMo tetrahedra,  a cornercorner with one S(8)V2GaMo tetrahedra,  a cornercorner with one S(12)VGaMo2 tetrahedra,  an edgeedge with one S(10)V2GaMo tetrahedra,  an edgeedge with one S(7)V2GaMo tetrahedra, and  an edgeedge with one S(1)V3Ga tetrahedra. In the fifth S site, S(5) is bonded to one V(3), one V(7), one Mo(2), and one Ga(1) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(10)V2GaMo tetrahedra,  a cornercorner with one S(1)V3Ga tetrahedra,  a cornercorner with one S(9)VGaMo2 tetrahedra,  an edgeedge with one S(11)V2GaMo tetrahedra,  an edgeedge with one S(8)V2GaMo tetrahedra, and  an edgeedge with one S(2)V3Ga tetrahedra. In the sixth S site, S(6) is bonded to one V(4), one V(8), one Mo(3), and one Ga(2) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(11)V2GaMo tetrahedra,  a cornercorner with one S(7)V2GaMo tetrahedra,  a cornercorner with one S(2)V3Ga tetrahedra,  an edgeedge with one S(3)V2GaMo tetrahedra,  an edgeedge with one S(12)VGaMo2 tetrahedra, and  an edgeedge with one S(9)VGaMo2 tetrahedra. In the seventh S site, S(7) is bonded to one V(1), one V(6), one Mo(1), and one Ga(2) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(11)V2GaMo tetrahedra,  a cornercorner with one S(6)V2GaMo tetrahedra,  a cornercorner with one S(2)V3Ga tetrahedra,  an edgeedge with one S(10)V2GaMo tetrahedra,  an edgeedge with one S(4)V2GaMo tetrahedra, and  an edgeedge with one S(1)V3Ga tetrahedra. In the eighth S site, S(8) is bonded to one V(2), one V(7), one Mo(2), and one Ga(3) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(3)V2GaMo tetrahedra,  a cornercorner with one S(4)V2GaMo tetrahedra,  a cornercorner with one S(12)VGaMo2 tetrahedra,  an edgeedge with one S(11)V2GaMo tetrahedra,  an edgeedge with one S(5)V2GaMo tetrahedra, and  an edgeedge with one S(2)V3Ga tetrahedra. In the ninth S site, S(9) is bonded to one V(8), one Mo(3), one Mo(4), and one Ga(1) atom to form distorted SVGaMo2 tetrahedra that share  a cornercorner with one S(10)V2GaMo tetrahedra,  a cornercorner with one S(5)V2GaMo tetrahedra,  a cornercorner with one S(1)V3Ga tetrahedra,  an edgeedge with one S(3)V2GaMo tetrahedra,  an edgeedge with one S(6)V2GaMo tetrahedra, and  an edgeedge with one S(12)VGaMo2 tetrahedra. In the tenth S site, S(10) is bonded to one V(1), one V(5), one Mo(1), and one Ga(1) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(5)V2GaMo tetrahedra,  a cornercorner with one S(1)V3Ga tetrahedra,  a cornercorner with one S(9)VGaMo2 tetrahedra,  an edgeedge with one S(4)V2GaMo tetrahedra,  an edgeedge with one S(7)V2GaMo tetrahedra, and  an edgeedge with one S(1)V3Ga tetrahedra. In the eleventh S site, S(11) is bonded to one V(2), one V(3), one Mo(2), and one Ga(2) atom to form distorted SV2GaMo tetrahedra that share  a cornercorner with one S(6)V2GaMo tetrahedra,  a cornercorner with one S(7)V2GaMo tetrahedra,  a cornercorner with one S(2)V3Ga tetrahedra,  an edgeedge with one S(5)V2GaMo tetrahedra,  an edgeedge with one S(8)V2GaMo tetrahedra, and  an edgeedge with one S(2)V3Ga tetrahedra. In the twelfth S site, S(12) is bonded to one V(4), one Mo(3), one Mo(4), and one Ga(3) atom to form distorted SVGaMo2 tetrahedra that share  a cornercorner with one S(3)V2GaMo tetrahedra,  a cornercorner with one S(4)V2GaMo tetrahedra,  a cornercorner with one S(8)V2GaMo tetrahedra,  an edgeedge with one S(3)V2GaMo tetrahedra,  an edgeedge with one S(6)V2GaMo tetrahedra, and  an edgeedge with one S(9)VGaMo2 tetrahedra. In the thirteenth S site, S(13) is bonded in a 3-coordinate geometry to one V(3), one V(6), and one Mo(4) atom. In the fourteenth S site, S(14) is bonded in a 3-coordinate geometry to one V(1), one V(4), and one V(7) atom. In the fifteenth S site, S(15) is bonded in a 3-coordinate geometry to one V(2), one V(5), and one V(8) atom. In the sixteenth S site, S(16) is bonded in a 3-coordinate geometry to one V(3), one V(6), and one Mo(1) atom. In the seventeenth S site, S(17) is bonded in a 3-coordinate geometry to one V(4), one V(7), and one Mo(2) atom. In the eighteenth S site, S(18) is bonded in a 3-coordinate geometry to one V(5), one V(8), and one Mo(3) atom. In the nineteenth S site, S(19) is bonded in a 3-coordinate geometry to one V(6), one Mo(1), and one Mo(4) atom. In the twentieth S site, S(20) is bonded in a 3-coordinate geometry to one V(1), one V(7), and one Mo(2) atom. In the twenty-first S site, S(21) is bonded in a 3-coordinate geometry to one V(2), one V(8), and one Mo(3) atom. In the twenty-second S site, S(22) is bonded in a 3-coordinate geometry to one V(3), one Mo(1), and one Mo(4) atom. In the twenty-third S site, S(23) is bonded in a 3-coordinate geometry to one V(1), one V(4), and one Mo(2) atom. In the twenty-fourth S site, S(24) is bonded in a 3-coordinate geometry to one V(2), one V(5), and one Mo(3) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_V8Ga3(MoS6)4
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   6.862
_cell_length_b   9.755
_cell_length_c   12.015
_cell_angle_alpha   65.655
_cell_angle_beta   72.932
_cell_angle_gamma   89.011
_symmetry_Int_Tables_number   1
_cell_volume   695.551
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  V  V0  1  0.412  0.006  0.192  1.0
  V  V1  1  0.746  0.339  0.525  1.0
  V  V2  1  0.931  0.536  0.140  1.0
  V  V3  1  0.271  0.865  0.474  1.0
  V  V4  1  0.604  0.198  0.808  1.0
  V  V5  1  0.791  0.395  0.999  1.0
  V  V6  1  0.128  0.723  0.334  1.0
  V  V7  1  0.463  0.058  0.666  1.0
  Ga  Ga8  1  0.004  0.999  0.000  1.0
  Ga  Ga9  1  0.338  0.332  0.333  1.0
  Ga  Ga10  1  0.672  0.665  0.665  1.0
  Mo  Mo11  1  0.207  0.400  0.998  1.0
  Mo  Mo12  1  0.530  0.735  0.333  1.0
  Mo  Mo13  1  0.863  0.069  0.666  1.0
  Mo  Mo14  1  0.071  0.669  0.864  1.0
  S  S15  1  0.728  0.136  0.000  1.0
  S  S16  1  0.061  0.469  0.333  1.0
  S  S17  1  0.396  0.803  0.666  1.0
  S  S18  1  0.578  0.438  0.848  1.0
  S  S19  1  0.909  0.773  0.183  1.0
  S  S20  1  0.242  0.106  0.515  1.0
  S  S21  1  0.426  0.287  0.151  1.0
  S  S22  1  0.757  0.621  0.484  1.0
  S  S23  1  0.092  0.956  0.817  1.0
  S  S24  1  0.275  0.136  0.000  1.0
  S  S25  1  0.607  0.470  0.334  1.0
  S  S26  1  0.940  0.804  0.665  1.0
  S  S27  1  0.735  0.626  0.004  1.0
  S  S28  1  0.084  0.958  0.333  1.0
  S  S29  1  0.419  0.292  0.666  1.0
  S  S30  1  0.909  0.286  0.173  1.0
  S  S31  1  0.234  0.617  0.511  1.0
  S  S32  1  0.567  0.950  0.844  1.0
  S  S33  1  0.083  0.452  0.825  1.0
  S  S34  1  0.411  0.795  0.156  1.0
  S  S35  1  0.745  0.128  0.489  1.0
  S  S36  1  0.261  0.632  0.005  1.0
  S  S37  1  0.590  0.972  0.333  1.0
  S  S38  1  0.922  0.305  0.666  1.0
[/CIF]
.